Microstructural evolution in copper subjected to severe ... 278.pdf Microstructural evolution in...
Embed Size (px)
Transcript of Microstructural evolution in copper subjected to severe ... 278.pdf Microstructural evolution in...
Acta Materialia 55 (2007) 13–28
Microstructural evolution in copper subjected to severe plastic deformation: Experiments and analysis
A. Mishra a, B.K. Kad b, F. Gregori c, M.A. Meyers a,*
a Department of Mechanical and Aerospace Engineering, Materials Science and Engineering Program, University of California,
San Diego, 9500 Gilman Drive, La Jolla, CA 92093-0411, USA b Department of Structural Engineering, University of California, San Diego, La Jolla, CA, USA
c Laboratoire des Propriétés Mécaniques et Thermodynamiques des Matériaux (CNRS), Université de Paris 13, France
Received 24 January 2006; received in revised form 14 July 2006; accepted 22 July 2006 Available online 27 October 2006
The evolution of microstructure and the mechanical response of copper subjected to severe plastic deformation using equal channel angular pressing (ECAP) was investigated. Samples were subjected to ECAP under three different processing routes: BC, A and C. The microstructural refinement was dependent on processing with route BC being the most effective. The mechanical response is modeled by an equation containing two dislocation evolution terms: one for the cells/subgrain interiors and one for the cells/subgrain walls. The deformation structure evolves from elongated dislocation cells to subgrains to equiaxed grains with diameters of �200–500 nm. The mis- orientation between adjacent regions, measured by electron backscatter diffraction, gradually increases. The mechanical response is well represented by a Voce equation with a saturation stress of 450 MPa. Interestingly, the microstructures produced through adiabatic shear localization during high strain rate deformation and ECAP are very similar, leading to the same grain size. It is shown that both pro- cesses have very close Zener–Hollomon parameters (lnZ � 25). Calculations show that grain boundaries with size of 200 nm can rotate by �30� during ECAP, thereby generating and retaining a steady-state equiaxed structure. This is confirmed by a grain-boundary mobil- ity calculation which shows that their velocity is 40 nm/s for a 200 nm grain size at 350 K, which is typical of an ECAP process. This can lead to the grain-boundary movement necessary to retain an equiaxed structure. � 2006 Acta Materialia Inc. Published by Elsevier Ltd. All rights reserved.
Keywords: Ultrafine grain metals; ECAP; Severe plastic deformation
In recent years, severe plastic deformation has been a topic of widespread research owing to its capability of pro- ducing ultrafine-grained materials. Indeed, three entire conferences, the NanoSPD series [1–3], were devoted entirely to this theme. This topic is reviewed by Furukawa et al. . Equal channel angular pressing (ECAP) is one of the variants of severe plastic deformation that is showing most promise because of its simplicity [5–8]. Grains of �200 nm with a fairly equiaxed distribution can be obtained using an optimized processing route.
1359-6454/$30.00 � 2006 Acta Materialia Inc. Published by Elsevier Ltd. All doi:10.1016/j.actamat.2006.07.008
* Corresponding author. Tel.: +1 858 534 4719. E-mail address: email@example.com (M.A. Meyers).
ECAP involves the use of a die that contains two inter- secting channels of equal cross-section. The strain that the sample experiences is dependent on two parameters: the inner angle of intersection of the channels, U, and outer angle of curvature, W . Among the incentives for using this technique, the most important one is that the sample cross-section remains unchanged during processing. The microstructure after a certain number of passes is strongly dependent on the rotation scheme [10–12]. The most widely used rotation schemes are: route A, where the billet is not rotated between consecutive passes; route BA, where the billet is rotated by 90� in alternate directions between con- secutive passes; route BC, where the billet is rotated by 90� in the same direction between consecutive passes; and route C, where the billet is rotated by 180� between consecutive
0 2 4 6 8 10 12 14 16
current results(hardness) Krishnaiah et al. Kadri et al. Wang et al. Vinogradov et al. Molodova et al. Langdon et al.(tension tests) Dalla Torre et al. Baik et al.
Number of passes
Fig. 1. Plot of hardness as a function of number of ECAP passes (data from different sources [21,25–30,72]).
14 A. Mishra et al. / Acta Materialia 55 (2007) 13–28
passes . Studies on samples produced by these rotation schemes have shown that route BC is the most effective route for producing an equiaxed microstructure [14,12,15,10]. However, it should be mentioned that con- flicting results have been reported (e.g. ).
There has been considerable recent effort devoted to defect structures and constitutive modeling of the response of copper to severe plastic deformation. These efforts have involved careful dislocation density measurements by Ungar, Zehetbauer and co-workers [17–19]. Based on this work, Goerdeler and Gottstein  and Baik et al. [21,22] developed constitutive equations including hardening con- tributions from both cell interior and walls. Goerdeler and Gottstein  considered both dislocation generation and annihilation. Toth et al.  developed a dislocation-based model for all hardening stages in large strain deformation that involved the evolution of the volume fraction of cell walls which decreases with the deformation and gives rise to a plateau-like behavior.
In spite of the large number of papers, over 100, dedi- cated to ECAP, little effort has been directed toward eluci- dating the mechanism of ultrafine grain formation. A notable exception is the recent work by Xu et al. . The research results presented herein had as a major goal the identification of the mechanisms of grain-size refinement.
2. Experimental methods
ECAP dies with two different values of / (the inner angle of channel intersection), 90� and 102�, were used for our experiments. As opposed to the widely used single piece or vertical split die, we used a design where the split was horizontal. This enabled replacement of the lower block with channels of different angles while the top piece was still reusable. In both dies, the outer arc of curvature, W, was 20�.
The shear strain per pass was equal to 0.87 for / = 102� and 1 for / = 90�. With the exception of the entry and exit points, the channel diameter was uniformly 0.95 cm. The diameter was slightly enlarged at the entry and exit points to permit easy reinsertion of the sample in the channel. The initial samples of commercially pure Cu (purity
0 0.02 0.04 0.06 0.08 0.1
initial 2passes 4passes 8passes initial(annealed)
Fig. 2. Compression test results for samples ranging from initial to 8 passes at a strain rate of 0.1/s.
0 0.1 0.2 0.3 0.4 0.5
Initial 2 passes 4 passes 8 passes
Strain rate =5*10-3/s Annealed samples
Fig. 3. Tensile test results of initial and ECAP samples. The samples were annealed at 700 �C for 1 h before processing.
A. Mishra et al. / Acta Materialia 55 (2007) 13–28 15
using route BC. As can be clearly seen, hardness saturates at eight passes. There is reasonable agreement between dif- ferent researchers. The results by Langdon et al.  are somewhat lower because we converted their yield stress (in tension) to hardness by multiplying it by 3. The satura- tion is connected to the lower limit of the grain size achieved by ECAP which seems to in the range of �200 nm. If one applies the Hall–Petch equation one can infer a grain size from the value of the yield stress. There is some variation in the literature regarding the Hall–Petch slope, and one obtains d = 690 nm from Feltham and Mea- kin , d = 428 nm from Gourdin and Lassila , d = 375 nm from Andrade et al. , and d = 67 nm from Armstrong . The above values are presented in Table 1.
Two initial conditions were used: an annealed and a work-hardened one. The results of compression tests are presented in Fig. 2. The two-pass sample showed a signifi- cant jump in strength over the initial sample. The rise in strength on higher number of passes was not as significant as it was for the first two passes. This is suggestive of the fact that the bulk of grain refinement happens in the first few passes. As will be discussed later, this was supported by EBSD data on grain size measurement distribution which yielded a steep decline in the grain size down to �200 nm on the first few passes while additional passes simply increased the fraction of grains in this size range. It was also observed that the effect of initial state of speci- men (annealed vs. cold worked) did not affect the mechan- ical response significantly. After two passes, the effects of initial microstructure are essentially eliminated.
Tensile tests were conducted on ECAP samples that were annealed at 700 �C for 1 h before processing. The ini- tial sample showed a large ductility. Work hardening in the process of severe plastic deformation caused a large decrease in ductility of the ECAP samples, as can be